(2) High-Speed Twin Roll Casting of Thin Aluminum Alloy Strips Containing Fe Impurities. from oscillating. Therefore, the addition of the nozzle also improves the strip surface. The nozzle precisely controls the solidiﬁcation length, which is not inﬂuenced by the bouncing of the meniscus on the melt surface; this allows for a uniform strip thickness. Thus, installing the nozzle improves heat transfer, the strip surface and the strip thickness. In order to increase the cooling rate, a copper roll was used instead of a steel roll. Because the thermal conductivity of copper is about eight times higher than that of steel, a copper roll is preferred for rapid solidiﬁcation. The roll diameter is 300 mm and the width is 100 mm. The roll is water-cooled from the inside. Lubricants become heat resistant between the roll and the melt and between the roll and the strip. Eliminating lubricant improves heat transfer. In the conventional twin roll caster for aluminum alloy (CTRCA), the lubricant is used to prevent the strip from sticking to the roll. However, a steel roll is used in the CTRCA and the temperature of the roll surface inﬂuenced the sticking behavior. The temperature of the copper roll surface is lower than that of the steel roll, so the copper roll temperature does not reach the threshold necessary for sticking. Therefore, the strip does not stick to the copper roll. The rolling load of the HSTRC is from ten to a hundred times smaller than that of the CTRCA. A small rolling load also helps to prevent the sticking of the strip. However, the rolling load of the HSTRC is large enough to obtain suﬃcient heat transfer between the roll and the strip. The rolling load should be set in the range of 0.1 to 0.5 kN/mm (per unit width). Low temperature casting was introduced in the HSTRC. When molten metal is poured from the crucible to the cooling slope, the superheat of the molten metal is 15 K. After passing through the cooling slope, the superheat is further decreased down to 5 K. The cooling slope is made from mild steel and is water-cooled from the inside. BN was sprayed on the surface of the cooling slope as a lubricant. The cooling slope length is 300 mm, the width is 100 mm, and the inclination angle is 60 degrees. 3.. Experimental Conditions. The 6111 aluminum alloy is one of the typical 6000 series alloys processed for automobile plates. The Fe content is restricted to less than 0.4 mass%. The Fe content of original 6111 is 0.13 mass%, and for these experiments, the Fe content was modiﬁed to 0.43, 0.62, 0.81 and 1.02 mass%. 2.7 kg of aluminum alloy was melted in an electric furnace. Before every casting, the roll surface was polished using #1200 emery paper. One roll was rigidly attached, while the other roll was supported by a spring. At the start of the casting, the roll gap was set at 1.0 mm and the roll gap varies along the strip thickness for the casting. The roll speed was set to 60 m/min. In comparison, the roll speed of CTRCA was slower than 10 m/min. Therefore, the proposed casting speed is very high. The rolling load was 0.14 kN/mm (per unit width). The mechanical properties of the strip were investigated using a tension test and a 180-degree bending test. The cast strip was cold rolled down to 0.5 mm, and T4 or T6 heat treatment was performed before the tension test. The 180-degree bending test was performed on a T4 heat treated. 2597. specimen at 1.0 mm thickness. The T4 and T6 heat treatment conditions are described below. For T4 heat treatment, the ascast strip was cold-rolled down to 0.5 or 1.0 mm without homogenization and intermediate annealing. The cold-rolled strip was kept at 813 K for four 14.4 ks, and then waterquenched. After T4, the strip was kept at 433 K for 21.6 ks. The gauge length and width was 20 and 10 mm, respectively, for the tension test piece. The microstructures of the as-cast and the T6 heat treated strip were metallographically observed. 4.. Results and Discussion. 4.1 Strip casting 6111 strip with Fe additions The original and modiﬁed 6111 were cast into the strip at a speed of 60 m/min. The roll casting ability increased as the Fe content increased. Continuity of the strip was improved by the addition of Fe. For the high-speed twin roll caster (HSTRC) used in the present study, casting of mushy solidiﬁcation type aluminum alloy was easier than skin formation solidiﬁcation type aluminum alloy. The modiﬁed 6111 became closer to the mushy solidiﬁcation type alloy as the Fe content was increased. This indicates that there is no problem in the high speed roll casting of recycled 6111. Figure 2 shows the surface of the as-cast strip. The width of the strip was the same as that of the roll. Ripple marks generated by the conventional twin roll caster for aluminum alloy (CTRCA) were not present on the surface. This is an advantage of the HSTRC. The oscillation of the meniscus was inhibited by the hydrostatic pressure of the molten metal. As a result, ripple marks did not occur. Fe content inﬂuenced the metallic luster of the strip surface. As the Fe content increased, the metallic luster decreased. This can be attributed to the strip temperature when it leaves the roll, which became respectively higher with increasing Fe content. The strip can not be cooled enough to exhibit metallic luster. However, there were no problems for continuously casting the modiﬁed 6111 strip. When the solidiﬁcation length was set longer, the strip surface exhibited metallic luster as the cooling time lengthened and the strip was suﬃciently cooled. The Fe impurities did not inﬂuence the strip surface. Figure 3 shows inﬂuence of Fe content on the strip thickness. The thickness decreased gradually as the Fe content increased. The reason for this was the improved ﬂuidity of the alloy in the semisolid condition as Fe content increased. However, the Fe content did not inﬂuence the thickness distribution of the strip cross-section. The as-cast strip could be cold-rolled down to 0.5 mm without homogenization or intermediate annealing. On the other hand, cracks occurred when the ingot cast using an insulator mold was cold-rolled without homogenization. This suggests that the roll-cast strip had good ductility due to the higher cooling rate used. The cooling rate of the strip cast by the HSTRC is estimated at about 4000 K/s near the surface, and about 1000 K/s in the middle of the thickness direction.4) The cooling rate of strips cast by the CTRCA was usually lower than 1000 K/s. Therefore, the cooling ability of the HSTRC is better than that of the CTRCA. No diﬀerences were apparent in the surfaces of the original 6111 strip and the modiﬁed 6111 strip after cold rolling, with both of these.
(3) 2598. T. Haga, M. Ikawa, H. Watari, K. Suzuki and S. Kumai. (b) 100mm. (a). (d). (c). (e). Strip thickness, d/mm. Fig. 2 Surface of as-cast strip of 6111 and Fe-added 6111 as model. (a) 0.13 mass% (b) 0.43 mass% (c) 0.62 mass% (d) 0.81 mass% (e) 1.02 mass%. 2.4. (a) 2.3. 2.2. 2.1. 0.5 mm. 2 0. 0.2. 0.4. 0.6. 0.8. 1. 1.2. Content of Fe (mass%). Fig. 3 Relationship between Fe content and strip thickness.. 20mm Fig. 4 0.5.. Surface of modiﬁed 6111 (1.5 mass%Fe) after cold rolling down to. surfaces exhibiting metallic luster. The surface of the strip after cold rolling is shown in Fig. 4. 4.2 Microstructure Figure 5 shows microstructure in cross-section of the as-. (b). Fig. 5 Microstructure of the cross-section of as-cast 6111 and Fe-added 6111 strip. (a) 6111 (0.13 mass%Fe) (b) Fe-added 6111 (1.02 mass%Fe). cast strip. It is clear that the microstructure created by the high cooling rate is very ﬁne. The microstructure is not uniform in the thickness direction. Speciﬁcally, the center area is diﬀerent from the other areas. The microstructure of the strip cast by CTRCA usually has a columnar structure. The HSTRC though, did not produce a columnar microstructure and there was no apparent interface in the center between the upper and lower solidiﬁcation layers like for the.
(4) High-Speed Twin Roll Casting of Thin Aluminum Alloy Strips Containing Fe Impurities. CTRCA. The level of Fe content did not aﬀect this tendency. The characteristics of the strip cast by the HSTRC are described below. An enlarged view of the microstructure cross-section is shown in Fig. 6. The microstructure of the center area resembled a spherical structure. This structure is typical for low superheat or low solidiﬁcation rate semisolid casting. The microstructure for the other areas was a duplex structure containing both dendritic and a globular structures. Globular crystals that existed in the dendritic structure were crystallized on the cooling slope. Figure 7 shows the grain interface of the ingot cast using the insulator mold and of the strip cast by HSTRC. Al–Fe–Si intermetallics were observed at the grain interface. However, there were not large Al–Fe– Si intermetallics found in the microstructure of the roll cast strip, like in the ingot cast metal. The intermetallics containing Fe in the roll cast strip became very small due to the high cooling rate. The HSTRC proved very capable of creating intermetallics with ﬁne impurities. Figure 8 shows. (a). 2599. (b). 50µ m (c). (d). Fig. 6 Enlarged view of microstructure of the cross-section in Fig. 5. (a) center area of Fig. 5(a), (b) near surface of Fig. 5(a) (c) center area of Fig. 5(b), (d) near surface of Fig. 5(b). (b). (a). 50 µ m. 10 µ m. Fig. 7 Intermetallic of as-cast strip and as cast ingot of 6111 including 1.02 mass%Fe. (a) as cast strip (b) as cast ingot. (b). (a). (d). (c). (e). 0.1mm Fig. 8 Microstructure of the cross-section of the strip after cold rolling and T6 heat treatment. (a) 0.13 mass%Fe (b) 0.43 mass%Fe (c) 0.62 mass%Fe (d) 0.81 mass%Fe (e) 1.02 mass%Fe.
(5) Si. 350. 35. 300. 30. 250. 25. 200. 20. 150. 15. 100 50. Ultimate tensile stress. 10. 0.2% yield stress. 5. Elongation (%). 5µm. 0.2% yield stress, σ0.2 /MPa. T. Haga, M. Ikawa, H. Watari, K. Suzuki and S. Kumai. Ultimate tensile stress, σ B /MPa. 2600. Elongation. 0 0. 0.2. 0.4. 0.6. 0.8. 1.0. 0 1.2. Fe content (mass%). Fig. 11 Tensile test results of T4 heat treatment strip.. Fe. Fig. 9 Result of line analysis of roll cast 6111 of 1.02 mass%Fe after cold rolling and T6 heat treatment.. 0.13mass%Fe 0.43mass%Fe 0.62mass%Fe. 40. 350 30. 300 250. 20. 200 150 Ultimate tensile stress. 100. 10. 0.2% yield stress. 50. Elongation (%). 0.2% yield stress, σ 0.2 /MPa. Ultimate tensile stress, σ B /MPa. 400. Elongation. 0.81mass%Fe 1.02mass%Fe Fig. 12 Outer surface of T4 heat treatment 1 mm-thick strip after 180degree bending.. 0. 0 0. 0.2. 0.4. 0.6. 0.8. 1. 1.2. Fe content (mass%). Fig. 10 Tensile test results of T6 heat treatment strip.. the microstructure after T6 heat treatment. The grain size was smaller than 20 mm and a diﬀerence in the microstructure between the center and the other areas of the as cast strip was resolved. A small non-uniformity of the microstructure in the thickness direction still existed. The intermetallic and the result of the line analysis are shown in Fig. 9. The Fe content of this specimen was 1.02 mass% and the intermetallic included Fe and Si. This was the Al–Fe–Si intermetallic. The intermetallic including Fe was smaller than 3 mm, and was not acicular but globular. Fe content inﬂuenced the number of the intermetallics but did not inﬂuence their size. The intermetallics became very small due to the rapid solidiﬁcation by the HSTRC and cold-rolling. The intermetallics were nearly uniformly distributed in the thickness direction. 4.3 Mechanical properties Mechanical properties were investigated using tensile tests and 180-degree bending tests. Figure 10 shows the tensile test results for the T6 heat-treated specimen. The ﬁgure shows that the tensile stress and proof stress were hardly inﬂuenced by Fe content. Si was used for the Al–Fe–Si intermetallic. Therefore, the amount of Mg2 Si precipitation might decrease. However, the tensile stress and the proof stress did not decrease. Cu2 FeAl7 might not be crystallized. by the eﬀect of -AlFeSi crystallization, therefore, the amount of precipitated Al2 CuMg might be suﬃcient for precipitation hardening. The elongation did not decrease when the Fe content was smaller than 0.8 mass% and the intermetallic including Fe did not reduce the elongation probably because of the very ﬁne size of the intermetallic, as shown in Fig. 9. Similarly, the addition of Fe did not produce any signiﬁcant diﬀerence in the tension test results for the T4 heat treated specimen. The tensile stress and proof stress increase gradually as Fe content increased and the grain size gradually became smaller as the Fe content increased. The grain size and intermetallics might inﬂuence the tensile stress and proof stress. However, the elongation did not decrease as the Fe content increased. Figure 11 shows the tensile test results for the T4 heat-treated specimen. The addition of Fe did not produce any signiﬁcant diﬀerence in the tension test results for the T4 heat treated specimen. The amount of the intermetallics including Fe might not inﬂuence the result of the tensile test as the intermetallics were very ﬁne. Figure 12 shows the bending test results. During the manufacturing of an automobile, the hemming process is performed of the end of the plate. It can be estimated whether a plate is suitable for hemming or not. The thickness of the strip was 1 mm and the heat treatment was T4. When the Fe content was smaller than 0.4 mass%, it exerted no inﬂuence on the outer surface conditions of the bent strip. When the content of Fe was larger than 0.5 mass%, cracking occurred on the outer surface the cracks however, were not deep.
(6) High-Speed Twin Roll Casting of Thin Aluminum Alloy Strips Containing Fe Impurities. enough to break the strip after bending. The cracking usually occurred on the outer surface after the 180-degree bending of 1 mm-thick 6111 plate of T4 heat treatment. Retrogressive heat-treatment was introduced to improve the cracking.5) Cracking, however, did not occur in the strip cast by the HSTRC when the Fe content was less than 0.4 mass%. The cast strip’s ability to withstand the hemming process was superior for those processed by the HSTRC than by the conventional process. This might be due to the eﬀect small grains and the intermetallics of the rapidly solidiﬁed strip generated by the HSTRC. This indicates the usefulness of the HSTRC for the 6000 alloy series and recycled 6000 alloy series used in automobiles. 5.. Conclusion. A strip of 6111 and 6111 with Fe-additions was processed by a high speed twin roll caster (HSTRC) at a speed of 60 m/ min. The 6111 aluminum alloy in which Fe was added as impurity up to a 1.0 Fe mass%, was used to model recycled aluminum alloy. Modiﬁed 6111 could be roll cast into strip. The Al–Fe–Si intermetallic of modiﬁed 6111 was very ﬁne due to the high cooling rate of the high speed twin roll caster.. 2601. When the Fe content was lower than 0.8 mass%, the tension test results of the Fe-added 6111 strip did not decrease. In addition, cracks did not occur on the outer surface after a 180degree bending test when the Fe content was lower than 0.5 mass%. This indicates that the high speed twin roll caster is suitable for improving the mechanical properties of recycled aluminum alloy. Acknowledgements This work was supported by RISTEX of JST (Japan Science and Technology Agency) and the Light Metal Foundation. REFERENCES 1) S. Kumai, K. Suzuki, Y. Saito and T. Haga: Trans. MRSJ. 29 (2004) 1817–1822. 2) T. Haga, M. Ikawa and S. Kumai: Trans. MRSJ. 29 (2004) 1823–1828. 3) T. Haga, K. Takahashi, M. Ikawa and H. Watari: J. Mater. Process. Tech. 153–154 (2004) 42–47. 4) K. Suzuki, S. Kumai, Y. Yuichi, A. Sato and T. Haga: Mater. Trans. 45 (2004) 403–406. 5) Aluminum International Today, Nov./Dec. (2002) 36..